Journal of Resea rch of the Notiona l Bureau of Standards Vol. 52, No. 4, April 1954 Research Paper 2492
Apparent Specific Volume of Polystyrene in Benzene, Toluene, Ethylbenzene, and 2-Butanone*
Maurice Griffel, ! Ralph S. Jessup, Joseph A. Cogliano,2 and Rita P. Park
:\1easurement s have been made a t t emperat ures near 27 and 30 C of t he den sities of pu rifi ed ben zene, to luene, ethylbenzene, a nd 2-but anone (methy lethylketone) , a nd of solutions of a purifi ed sample of p olysty r ene in t hese solven ts. 'Wi thi n t he precision of t he meas urements (abou t 1 or 2 in 105 density) t he appa ren t specific volume of the poly-styrene is a constan t independ ent of t he concen t rat ion in a nyone solvent, bu t d epends to so me exten t upon t he solven t . The lowes t values, which were obtained wi t h 2-bu tanone, a l'e a bout 1 p ercent lower t han t he hi ghest val ues, \ V hi ch were obt ained wit h ethylbe nzene . The va lu es are a ll lower t han t hose of th e vir t ua l liquid polym er , ob tained by extrapolation of data on specifi c volume above t he glass t ra nsi t ion temperature, although t he data of o t her obser vers indi ca te t hat t his is n ot t ru e for all solvents. I n a ll fo ur solven t s t he cha nge of t he appa ren t specific volume wi t h temp erature is less t han fo r t he liq uid p olym er.
The changes in volume upon mi xin g of polystyr ene wi t h t he solven ts are shown to have a signifi cant cffect on s uch then nod.vna mi c proper t ics as heat , Free energy , a nd cnt ropy of mix ing .
Theoretical t rea tmen ts of the thermodynamics of polymer solutions arc usually based on assumptions that imply that there is no vol ume change on mixing of polymers and solvents. Experimen tally, however , it is found that there is a small but measumble change in volme when mixing takes place at constan t pl'essul'e [1 , 2, 3, 4, II , 12, 15].3 Because a change in volume will affect the experimen tally determined values of such thermodynamic quantities as heat, free energy, and en tropy of mixing at constant pl'ess me  , a knowl edge of the magni t ude of the change in volume is of impor tance in comparing experimen tal r esul ts wi th theoretical predic tions. The work described in thi s paper was under taken to provid e data to a id in interpreting the resul ts of measurements of heats of mixing of polymers and solven ts .
The polystyrene used was obtained from the Dow Chemical Co. through the courtesy of R. F. Boyer . I t had been prepared by thermal polymerization with-ou t catalyst a t 1800 C. After receip t of the material it was purified as follows: 150 g of polystyrene was dissolved in abou t 750 ml of benzene, and was then precipitated by pouring the solution slowly into about 3 li ters of well-stirred methanol. After allow-ing the precipit a te to set tle, the liquid was decanted. This procedure was r epeated twice. The polystyrene \vas then dissolved in 2 li ters of benzene, the mixt ure was frozen at - 300 C. and most of the benzene was removed by evac uation at tempera tures no t ex-ceeding 3 C. E vac uation was continued at a
*'l' bis work was s ll pporicd in par t by t he Heconstruction Finance Corpora t ion , Office of Syn thetic Rubber, in connection with t he Go\'ernment Synthetic R ubbcr Program.
1 Presen t address, Th l' John s rropki ll s Univf' l's it y , Baltimo re, IVfd . 2 Present address, George \ Vashin gloll U niversit y. \ Vashillgto n, D . C . 3 Figures in brackets indicate the li terature rererences at the end or this paper.
temperat Lll'e of 70 C for about 10 days . Tlw temperat Lll'e was then gradually increased to 1200 C over a period of about a week, and the pressure over the material was maintained a t less th an 10-" mm of mercll1'y . As a resul t of this treatmen t, the polystyrene was fu sed in to a solid mass. To facili ta te subsequen t h andling, i t was ground in a cu t ting mill , so that the final product consis ted of part icles abou t 3 mm or less in diam eter .
From observations of ligh t scattering the values M = 190,000 and B = 5.2 X 10 - 4 cgs uni t were ob-tained for weigh t average molecular weigh t and second viri al coefficient, respectively , for the purified polymer .4
The volatile constituen ts of th e purified polymer were determined 5 by hea ting a crushed sample to 150 to 1600 C for 2 hI' in a previously evacuated space of known volume, measuring the resulting in-crease in pressure, and making a mass spectrometric analysis of th e gas evolved . The amoun ts of volatile constituen ts found in this way, expressed in percen t-age of the total ,veigh t of polymer , are as follows :
WateL _____ ______ _____________ ___ _ Carbon dioxide ___ . _______ _________ _ Benze ne ___ ___ ___ _________________ _
T otal volat ile impuritic,L ___ ____ _
Percen tage by weigh t
O. 101 . 021 . 014
The fact tha t appreciable amounts of volatile impu -rities remained after prolonged h eating and evacua-tion, as described above, is in accord with the find-ings of Grassie  in regard to the difficulty of re-moving volatile impurities from polymers .
Tbese values were obtained by M . Wales or thc Pol ymer Structure Section of tbe Bureau.
, In tbe Mass Spectrometry Section of the Bureau.
The benzene used was purified 6 by frac tional freezing. The other solvents were purified by distil-lation. Freezing-curve measurements 7 indicated a purity of 99.65 and 99.80 mole percent for the toluene and 2-butanone, respectively. The other solvents are believed to be of comparable purity, although no actual determinations of their purity were made. Although impurities in the solvents would affect the densities of both solvents and solutions, it seems very improbable that they would affect the apparent specific volume of the solute to an appreciable extent in view of the small differences between the values for apparent specific volume in different solvents . In table 1 the observed densities of the three hydro-carbon solvents are compared with "best" values of t.hese properties derived from data reported in the literature .
TAB L E 1. Den sities of hydTocaI'bon solvents
DenSity, g/cm" at-
Solvent 26.890 C 29.971 C
Literature Observed Literature Observed values values values values
Benzenc ____ ___________ 0. 87167 0.87165 0.86840 0.86834 Toluene ________________ . 86052 .86035 . 85766 . 8,)747 E thylbenzene __________ .86096 . 86123 .85826 ,85851
3 . Apparatus and Method
Densities of solvents and solutions of known com-position were measured by means of picnometers, and values of apparent specific volume of polystyrene were calculated from the data.
The Pyrex picnometers used (A, fig . 1) are of the bicapillary type described by Heller and Thompson  . The capillaries were of "precision-bore" quality, and before sealing to the picnometers they were calibrated by measuring at X-in . intervals the length of a weighed mercury thread. They were found to have a uniform radius of 0.494 mm:
The completed picnometers had volumes of about 22 cm3 and were calibrated by weighing when empty and when filled with double-distilled water  at temperatures near 27 and 30 C. The values for the density of water were calculated from an equation derived by Tilton and Taylor  to represent the data of Chappuis . Weighings were made to 0.1 mg or better on an Ainsworth semimicrobalance, using newly calibrated weights. Final weighings were made after allowing ample time for the attain-ment of temperature equilibrium in the balance. Two picnometers were used in the measurements, and a third was used as a tare in weighing. All weights were corrected for air buoyancy on the basis of observations of barometric pressure, temperature in the balance case, and relative humidity.
By T . M. Mears of the Engine Fuels Section of the Bureau, 7 By G. T . Fw-ukawa of the Thermodynamics Section of the Bureau.
The positions of the two menisci relative to refer-ence marks on the capillaries were read to 0.01 mm by means of a Gaertner traveling microscope. Dur-ing these readings the picnometers were immersed in a water bath whose temperature during an experi-ment was maintained constant within about 0.002 deg C. The wall of the bath through which the menisci were observed was of plate glass. The temperature of the bath was measured by means of a strain-free platinum resistance thermometer and a special Mueller bridge.
The solutions were made up in 60 ml bottles with ground-glass stoppers as follows: A clean bottle con-taining a Pyrex-glass sealed stirring rod for use with a magnetic stirrer was weighed with its stopper, using a similar bottle for a tare. A sample of poly-styrene of approximately known weight was then introduced into the bottle through a funnel in such a manner as to avoid getting any polystyrene on the ground-glass joint, and the bottle was again weighed. A measul'ed amount (usually 50 ml) of solvent was introduced into the bottle, which was then closed with the ground-glass stopper . In handling the bot-tle great care was taken to avoid getting any solution on the ground-glass joint. The bottle was then placed on the magnetic stirrer, and stirring was con-tinued until a uniform solution was obtained. When mixing was complete some solvent had condensed in the upper part of the bottle, in the ground-glass joint, and the inside of the stopper. This condensed sol-vent was removed by drawing clean dry air over these areas, and the stopper was replaced. The two empty picnometers were then weighed; following this , the bottle containing the solution was weighed, and the solution was transferred to the picnometers as de-scribed in the following para